1.1 This standard practice provides methodology to convert fracture strength parameters (primarily the mean strength and the Weibull characteristic strength) estimated from data obtained with one test geometry to strength parameters representing other test geometries. This practice addresses uniaxial strength data as well as some biaxial strength data. It may also be used for more complex geometries proved that the effective areas and effective volumes can be estimated. It is for the evaluation of Weibull probability distribution parameters for advanced ceramics that fail in a brittle fashion. Fig. 1 shows the typical variation of strength with size. The larger the specimen or component, the weaker it is likely to be.

1.2 As noted in Practice C1239, the failure strength of advanced ceramics is treated as a continuous random variable. A number of functions may be used to characterize the strength distribution of brittle ceramics, but the Weibull distribution is the most appropriate especially since it permits strength scaling for the size of specimens or component. Typically, a number of test specimens with well-defined geometry are broken under well-defined loading conditions. The force at which each test specimen fails is recorded and fracture strength calculated. The strength values are used to obtain Weibull parameter estimates associated with the underlying population distribution.

1.3 This standard is restricted to the assumption that the distribution underlying the failure strengths is the two-parameter Weibull distribution with size scaling. The practice also assumes that the flaw population is stable with time and that no slow crack growth occurs.

Advanced ceramics usually display a linear stress-strain behavior to failure. Lack of ductility combined with flaws that have various sizes and orientations typically leads to large scatter in failure strength. Strength is not a deterministic property but instead reflects the intrinsic fracture toughness and a distribution (size and orientation) of flaws present in the material. This standard is applicable to brittle monolithic ceramics which fail as a result of catastrophic propagation of flaws. Possible rising R-curve effects are also not considered, but are inherently incorporated into the strength measurements.

Two- and three-parameter formulations exist for the Weibull distribution. This standard is restricted to the two-parameter formulation.

Tensile and flexural test specimens are the most commonly used test configurations for advanced ceramics. Ring-on-ring and pressure-on-ring test specimens which have multi-axial states of stress are also included. Closed-form solutions for the effective volume and effective surfaces and the Weibull material scale factor are included for these configurations. This practice also incorporates size scaling methods for C-ring test specimens for which numerical approaches are necessary. A generic approach for arbitrary shaped test specimens or components that utilizes finite element analyses is presented in Annex A3.

The fracture origins of failed test specimens can be determined using fractographic analysis. The spatial distribution of these strength controlling flaws can be over a volume or an area (as in the case of surface flaws). This standard allows for the conversion of strength parameters associated with either type of spatial distribution. Length scaling for strength controlling flaws located along edges of a test specimen is not covered in this practice.

The scaling of strength with size in accordance with the Weibull model is based on several key assumptions (5). It is assumed that the same specific flaw type controls strength in the various specimen configurations. It is assumed that the material is uniform, homogeneous, and isotropic. If the material is a composite, it is assumed that the composite phases are sufficiently small that the structure behaves on an engineering scale as a homogeneous and isotropic body. The composite must contain a sufficient quantity of uniformly-distributed, randomly-oriented, reinforcing elements such that the material is effectively homogeneous. Whisker-toughened ceramic composites may be representative of this type of material. This practice is also applicable to composite ceramics that do not exhibit any appreciable bilinear or nonlinear deformation behavior. This standard and the conventional Weibull strength scaling with size may not be suitable for continuous fiber-reinforced composite ceramics. The material is assumed to fracture in a brittle fashion, a consequence of stress causing catastrophic propagation of flaws. The material is assumed to be consistent (batch to batch, day to day, etc.). It is assumed that the strength distribution follows a Weibull two parameter distribution. It is assumed that each test piece has a statistically significant number of flaws and that they are randomly distributed. It is assumed that the flaws are small relative to the specimen cross section size. If multiple flaw types are present and control strength, then strengths may scale differently for each flaw type. Consult Practice C1239 and the example in 9.1 for further guidance on how to apply censored statistics in such cases. It is also assumed that the specimen stress state and the maximum stress are accurately determined. It is assumed that the actual data from a set of fractured specimens are accurate and precise. (See Terminology E456 for definitions of the latter two terms.) For this reason, this standard frequently references other ASTM standard test methods and practices which are known to be reliable in this respect.

Even if test data has been accurately and precisely measured, it should be recognized that the Weibull parameters determined from test data are in fact estimates. The estimates can vary from the actual (population) material strength parameters. Consult Practice C1239 for further guidance on the confidence bounds of Weibull parameter estimates based on test data for a finite sample size of test fractures.

When correlating strength parameters from test data from one specimen geometry to a second, the accuracy of the correlation depends upon whether the assumptions listed in 5.5 are met. In addition, statistical sampling effects as discussed in 5.6 may also contribute to variations between computed and observed strength-size scaling trends.

There are practical limits to Weibull strength scaling that should be considered. For example, it is implicitly assumed in the Weibull model that flaws are small relative to the specimen size. Pores that are 50 μm (0.050 mm) in diameter are volume-distributed flaws in tension or flexural strength specimens with 5 mm or greater cross section sizes. The same may not be true if the cross section size is only 100 μm.

Tile in English: Standard Practice for Size Scaling of Tensile Strengths Using Weibull Statistics for Advanced Ceramics

- ASTM E2214-2008e1 Standard Practice for Specifying and Verifying the Performance of Color-Measuring Instruments
- ASTM G181-2004(2009) Standard Practice for Conducting Friction Tests of Piston Ring and Cylinder Liner Materials Under Lubricated Conditions
- ASTM A799/A799M-2004(2009) Standard Practice for Steel Castings, Stainless, Instrument Calibration, for Estimating Ferrite Content
- ASTM D61-1975(2010) Standard Test Method for Softening Point of Pitches (Cube-in-Water Method)
- ASTM D2244-2009b Standard Practice for Calculation of Color Tolerances and Color Differences from Instrumentally Measured Color Coordinates
- ASTM D4597-2003(2009)e1 Standard Practice for Sampling Workplace Atmospheres to Collect Gases or Vapors with Solid Sorbent Diffusive Samplers
- ASTM D4308-1995(2010) Standard Test Method for Electrical Conductivity of Liquid Hydrocarbons by Precision Meter
- ASTM D4995-2004(2010) Standard Specifications for Electronic and Degreasing Grades of 1,1,2-Trichloro 1,2,2,-Trifluoroethane Solvent
- ASTM D7504-2009e1 Standard Test Method for Trace Impurities in Monocyclic Aromatic Hydrocarbons by Gas Chromatography and Effective Carbon Number
- ASTM D7123-2004(2010) Standard Practice for Handling, Transportation, and Storage of HCFC Blend B (CF inf 3 /inf CCl inf 2 /inf H, Ar, and CF inf 4 /inf )

- ASTM A296-1968 standard specification for corrosion-resistant iron-chromium,iron-chromium-nickel,and nickel base alloy castings for general application
- ASTM A510/A510M-2011 standard specification for general requirements for wire rods and coarse round wire, carbon steel, and alloy steel
- ASTM B840-1999(2009) Standard Specification for Electrodeposited Coatings for Zinc Cobalt Alloy Deposits
- ASTM B842-1999(2005) Standard Specification for Electrodeposited Coatings for Zinc Iron Alloy Deposits
- ASTM C1061-1986 standard test method for thermal transmission properties of nonhomogeneous insulation panels installed vertically
- ASTM D1024-1959 method of test for butadiene dimer and styrene in butadiene concentrates withdrawn 1969
- ASTM D1117-1980 standard methods of testing nonwoven fabrics
- ASTM D2369-2010 standard test method for volatile content of coatings
- ASTM D6577-2006 Standard Guide for Testing Industrial Protective Coatings
- ASTM E1699-2010 standard practice for performing value analysis (va) of buildings and building systems and other constructed projects
- ASTM F795-1982 standard practice for determining the performance of a filter medium employing a single-pass,constant- rate,liquid test
- ASTM G85-2011 standard practice for modified salt spray (fog) testing
- ASTM D4329-2013 Standard Practice for Fluorescent Ultraviolet (UV) Lamp Apparatus Exposure of Plastics
- ASTM F21-1965(1996) Standard Test Method for Hydrophobic Surface Films by the Atomizer Test
- ASTM D2578-2004 Standard Test Method for Wetting Tension of Polyethylene and Polypropylene Films

- ASTM E2843-2016 Standard Specification for Demonstrating That a Building is in Walkable Proximity to Neighborhood Assets
- ASTM A276/A276M-2016 Standard Specification for Stainless Steel Bars and Shapes
- ASTM A479/A479M-2016 Standard Specification for Stainless Steel Bars and Shapes for Use in Boilers and Other Pressure Vessels
- ASTM A1044/A1044M-2016 Standard Specification for Steel Stud Assemblies for Shear Reinforcement of Concrete
- ASTM E2469-2016 Standard Test Method for Chloride in Mono-,Di- and Tri-ethylene Glycol by Ion Chromatography
- ASTM E1354-2016 Standard Test Method for Heat and Visible Smoke Release Rates for Materials and Products Using an Oxygen Consumption Calorimeter
- ASTM F2848-2016 Standard Specification for Medical-Grade Ultra-High Molecular Weight Polyethylene Yarns
- ASTM C192/C192M-2016 Standard Practice for Making and Curing Concrete Test Specimens in the Laboratory
- ASTM D4029/D4029M-2016 Standard Specification for Finished Woven Glass Fabrics
- ASTM C753-2016 Standard Specification for Nuclear-Grade,Sinterable Uranium Dioxide Powder
- ASTM D4389/D4389M-2016 Standard Specification for Finished Glass Fabrics Woven From Rovings
- ASTM C138/C138M-2016 Standard Test Method for Density (Unit Weight),Yield,and Air Content (Gravimetric) of Concrete
- ASTM D7679-2016 Standard Test Method for Sulfur Content in Carbon Black Feedstock Oils
- ASTM C1542/C1542M-2016 Standard Test Method for Measuring Length of Concrete Cores
- ASTM D7846-2016 Standard Practice for Reporting Uniaxial Strength Data and Estimating Weibull Distribution Parameters for Advanced Graphites